Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics


 Dora Hicks
 1 years ago
 Views:
Transcription
1 /j x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department of Mechanical Construction and Production, SintPietersnieuwstraat 41, 9000 Gent, Belgium Received in final form 10 October 2006 ABSTRACT Even if the extent of damage in fibrereinforced plastics is limited, it already affects the elastic properties. Therefore, the damage initiation and propagation in composite structures is monitored very carefully. Beside the use of nondestructive testing methods (ultrasonic inspection, optical fibre sensing), the followup of the degradation of engineering properties such as the stiffness is a common approach. In this paper, it is investigated if the Poisson s ratio can be used as a sensitive indicator of (fatigue) damage in fibrereinforced plastics. Static, cyclic and fatigue tests have been performed on [0 /90 ] 2s glass/epoxy laminates, and axial and transverse strain were measured continuously. The evolution of the Poisson s ratio versus time and axial strain is studied. It is concluded that the degradation of the Poisson s ratio can be a valuable indicator of damage, in combination with the stiffness degradation. Keywords damage mechanics;fatigue;finite element analysis;polymermatrix composites (PMCs). INTRODUCTION Damage in fibrereinforced composites can take many forms: 1,2 (i) matrix cracks, (ii) fibrematrix interface failure, (iii) fibre pullout, (iv) delaminations and (v) fibre fracture. This damage affects the value of the elastic properties at an early stage. Especially in fatigue, the damage initiation phase can cause a pronounced drop of the elastic modulus of 5 10%. In the next damage propagation phase, the stiffness continues to decrease gradually, ranging from a few percent for unidirectionally reinforced carbon composites to several tens of percents for multidirectional glass laminates. 3 7 Most onedimensional damage models for fibrereinforced composites only account for the effect of damage on the stiffness The degradation of the Poisson s ratio is not included in these models. Nevertheless this degradation has been observed and is not negligible. 17,18 Bandoh et al. showed that the Poisson s ratio of a carbon/epoxy UD laminate can drop by 50% under static tensile loading, 17 while Pidaparti and Vogt proved that the Poisson s ratio is a very sensitive parameter whilst monitoring fatigue damage in human bone. 18 In this paper, it is investigated whether or not the Poisson s ratio can be used as a sensitive indicator of (fatigue) Correspondence: W. Van Paepegem. damage in fibrereinforced composites for both static, cyclic and fatigue loading. Just like the stiffness, it can be measured accurately and nondestructively. Further, it gives information about the damage state of the offaxis plies in a multidirectional composite laminate. For longterm measurements, the use of strain gauges is less appropriate, but optical fibre sensor pads can be a viable alternative. In a first step, static tensile tests are performed on [0 /90 ] 2s glass/epoxy laminates, followed by cyclic loadingunloading tests and straincontrolled fatigue tests. MATERIAL AND TEST METHODS The material under study was a glass/epoxy composite. The glass reinforcement was a unidirectional Eglass fabric (Roviglas R17/475). In the fibre direction e 11, the reinforcement was 475 g/m 2, while in the direction e 22,the reinforcement was 17 g/m 2. The epoxy matrix was Araldite LY 556. Three stacking sequences were manufactured: [0 ] 8, [90 ] 8 and [0 /90 ] 2s with the angle referred to the direction e 11. The layups [0 ] 8 and [90 ] 8 were used for characterization in the orthotropic material directions, while [0 /90 ] 2s was used for the study of the Poisson s ratio. 269
2 270 W. VAN PAEPEGEM et al. All specimens were manufactured by vacuum assisted resin transfer moulding with a closed steel mould. The nominal thickness of all specimens was 3.0 mm and the fibre volume fraction was between 48 and 50%. The samples were cut to dimensions on a watercooled diamond tipped saw. The inplane elastic properties of the individual glass/epoxy lamina were determined by the dynamic modulus identification method described by Sol et al. 19,20 and are listed in Table 1. Apart from the dynamic modulus identification method, static tensile tests on the [0 ] 8 and [90 ] 8 layups have been performed to check the values of the elastic properties and to determine the static strengths. It is important to mention that the mechanical behaviour in the e 11 and e 22 direction is linear until failure. The tensile strength properties were determined from the [0 ] 8 and [90 ] 8 stacking sequence and are listed in Table 2. Based on this characterization of the individual glass/epoxy lamina, [0 /90 ] 2s crossply laminates were manufactured for investigation of the Poisson s ratio. STATIC MEASUREMENTS OF The elastic and strength properties of the [0 /90 ] 2s laminate were determined by quasistatic tensile tests on an Table 1 Inplane elastic properties of the individual glass/epoxy lamina E 11 (GPa) 38.9 E 22 (Gpa) 13.3 ν 12 [ ] G 12 (Gpa) 5.13 Table 2 Tensile strength properties of the individual glass/epoxy lamina X T (Mpa) ε11 ult [ ] Y T (Mpa) 36.5 ε22 ult [ ] Instron electromechanical testing machine. The tensile tests were displacementcontrolled with a displacement speed of 1 mm/min. The specimen geometry is illustrated in Fig. 1. The nominal specimen width was 34 mm and the thickness 3 mm. The gauge length was 140 mm. Two strain gauges were applied in the X and Y direction. The tests were done in accordance with ASTM D3039 Standard Test Method for Tensile Properties of Polymer Matrix Composite Materials. Figure 2 shows the stress strain curve for the [0 /90 ] 2s specimens IF4 and IF6. In the first measurement, the strain gauge signal was lost at about 1.0% longitudinal strain (due to debonding), but the load signal was measured until failure. The calculated failure stresses were and Mpa, respectively. The failure strain of specimen IF6 was (or 2.08%). The value of the elastic modulus was and GPa, respectively (determined by leastsquares linear fit for the strain range [0;0.0025]). The value measured by the dynamic modulus identification method was GPa for another specimen from the same batch of material. At a level of about 100 MPa axial stress, there is a small change in slope of the stress strain curve. The corresponding strain is slightly higher than (0.25%) which is the fracture strain of the 90 plies in the crossply laminate (see Table 2). The corresponding history of the Poisson s ratio versus is shown in Fig. 3. Although the axial stress strain curve is almost linear (Fig. 2), the Poisson s ratio is decreasing quite fast. This is due to early transverse matrix cracking of the 90 plies. Indeed the failure strain ε22 ult of the 90 plies equals only (see Table 2) and once the axial strain in these plies exceeds this threshold, the 90 plies are severely cracked. The estimated value of in the elastic regime is and 2 for IF4 and IF6, respectively. The calculated value of from the dynamic modulus identification method is The latter method is a mixed numerical/experimental method that aims to identify the engineering constants of orthotropic materials using measured resonant frequencies of freely suspended rectangular specimens. For the identification of the four orthotropic material constants, it is necessary 3 mm Y θ= 0 X Fig. 1 [0 /90 ] 2s glass/epoxy specimen s layout.
3 POISSON S RATIO AS AN INDICATOR OF DAMAGE 271 Stressstrain curve for static [0 /90 ] 2s tests IF4 and IF6 Forcedisplacement curve for cyclic [0 /90 ] 2s test IF3 500 IF4 IF6 = GPa σ xx [MPa] = GPa Force [kn] Fig. 2 Stress strain curve for the static tensile test of the [0 /90 ] 2s specimens IF4 and IF Displacement [mm] Fig. 4 Forcedisplacement curve for the [0 /90 ] 2s specimen IF3. Time history of and ε yy for cyclic [0 /90 ] 2s test IF versus for static [0 /90 ] 2s tests IF4 and IF6 static [0 /90 ] 2s test IF4 static [0 /90 ] 2s test IF ε yy and ε yy Fig. 3 Evolution of the Poisson s ratio in function of the longitudinal strain for the [0 /90 ] 2s specimens IF4 and IF6. to measure the first three resonant frequencies of a rectangular plate and the first resonant frequency of two beams, one cut along the longitudinal direction and the other cut along the transversal direction. Starting from an initial guess, the engineering constants are iteratively updated till a series of numerically computed resonance frequencies match the experimentally measured frequencies. This method is completely nondestructive which can explain the higher value for the Poisson s ratio. MEASUREMENTS OF UNDER CYCLIC LOADING In order to observe the behaviour of the Poisson s ratio under repeated loading, cyclic tensile tests are performed Time [s] Fig. 5 Time history of and ε yy for the [0 /90 ] 2s specimen IF3. The displacement speed is 2 mm/min and the load cycles between 1 kn and subsequent load levels of 20, 20, 25, 35, 35, 42, 45, 48 and 54.7 kn (failure load), as shown in Fig. 4. The small change of the slope in the curve at 10 kn corresponds with a longitudinal stress σ xx of MPa. This kneepoint could indeed be observed in the stress strain curves in Fig. 2. The corresponding time history of the measured longitudinal strain and the transverse strain ε yy for the cyclic tensile test on the [0 /90 ] 2s specimen IF3 is shown in Fig. 5. At the lowest loads of 1 kn, the transverses strain ε yy becomes slightly positive. This is not caused by improper calibration of the strain gauges. The strain measurement channels are calibrated for each strain gauge with a precision shunt resistance. It will be shown in subsequent figures that this effect is very reproducible. Both the failure stress and failure strain are higher than in the quasistatic tensile tests. The failure stress here is
4 272 W. VAN PAEPEGEM et al. Time history of and for cyclic [0 /90 ] 2s test IF3, Time [s] Fig. 6 Time history of the Poisson s ratio for the [0 /90 ] 2s specimen IF3. Fig. 8 Instrumentation of the [0 /90 ] 2s glass/epoxy specimens. versus for cyclic [0 /90 ] 2s test IF3 cyclic [0 /90 ] 2s test IF3 static [0 /90 ] 2s test IF4 static [0 /90 ] 2s test IF6 value must be stress dependent because no further damage occurs during unloading. νxy Fig. 7 Evolution of the Poisson s ratio in function of the longitudinal strain for the cyclic [0 /90 ] 2s test IF MPa and the failure strain (or 2.93%). This strengthening effect might be due to better fibre alignment. A similar phenomenon was already reported by the authors for cyclic loading/unloading tests of [+45/ 45] 2s glass/epoxy laminates. 21,22 Figure 6 shows the corresponding time history of the Poisson s ratio. In the region of low forces (and thus low strains ), the Poisson s ratio becomes negative, due to the slightly positive value of the transverse strain ε yy for small loading values (see Fig. 5). In Fig. 7, the evolution of the Poisson s ratio is plotted against the longitudinal strain, together with its evolution in the quasistatic tensile tests IF4 and IF6 (see Fig. 3). It can be clearly seen that the maxima of the cyclic curves follow the static curve very well. As the Poisson s ratio changes drastically during unloading, its MEASUREMENTS OF UNDER FATIGUE LOADING In order to assess the sensitivity of the Poisson s ratio for fatigue damage, tension tension fatigue tests have been conducted on the same material. The specimen geometry was the same as shown in Fig. 1, but the longitudinal strain gauge has been replaced by an extensometer. The fatigue tests were straincontrolled, so that the measurement of the transverse strain ε yy immediately yields the value of the Poisson s ratio. The maximum strain level was chosen (0.6%), because this strain level is slightly higher than the kneepoint in the static stress strain curve (see Fig. 2). Using a strain ratio R of 0.1 (similar to the stress ratio in fatigue), the minimum strain level is (0.06%). The fatigue tests were done at 2 Hz on an Instron servohydraulic testing machine. Figure 8 shows the clamped specimen with its instrumentation. The extensometer measures the longitudinal strain, the transverse strain gauge measures the transverse strain and a thermocouple monitors the surface temperature of the composite laminate. Load and displacement were measured by the servohydraulic machine control. Normally, the life time of strain gauges in fatigue is very limited, because the limit strain levels they can endure in fatigue, are very much reduced compared to static operation. However, in this case the transverse strain levels were very small (a few hundred microstrains) and no temperature rise of the surface was detected from the thermocouple.
5 POISSON S RATIO AS AN INDICATOR OF DAMAGE 273 Stressstrain curve for [0 /90 ] 2s fatigue test W_090_7 versus for [0 /90 ] 2s fatigue test W_090_ = GPa static [0 /90 ] 2s test IF4 static [0 /90 ] 2s test IF6 [0 /90 ] 2s fatigue test W_090_7: cycle [0 /90 ] 2s fatigue test W_090_7: cycle [0 /90 ] 2s fatigue test W_090_7: cycle σ xx [MPa] = GPa static [0 /90 ] 2s test W_090_7: cycle 0 intermediate static [0 /90 ] 2s test W_090_7: cycle Fig. 9 Stress strain curve for the initial and intermediate static tensile tests of the [0 /90 ] 2s fatigue test W Fig. 11 Evolution of the Poisson s ratio in function of the longitudinal strain for the 0 /90 ] 2s specimen W at three chosen intervals in the fatigue test versus time for [0 /90 ] 2s fatigue test W_090_7 [0 /90 ] 2s fatigue test W_090_7: cycle [0 /90 ] 2s fatigue test W_090_7: cycle [0 /90 ] 2s fatigue test W_090_7: cycle Time Fig. 10 Time history of the Poisson s ratio for the [0 /90 ] 2s specimen W at three chosen intervals in the fatigue test. The signals of load, displacement, extensometer, strain gauge and temperature were each sampled at 100 Hz every 5 min for five subsequent loading cycles with a National Instruments NI DAQPAD 6052E measurement card and LabVIEW software. For the first fatigue test W 090 7, 7500 loading cycles were applied. The stress strain curve was measured before fatigue testing, but only to a very low axial strain of (0.1%), because the failure strain of the 90 plies is only (0.25%) (see Table 2). After stopping the fatigue test, the same static tensile test was repeated. Figure 9 shows the measured static stress strain curves for cycle 0 and cycle A degradation of the axial stiffness is observed from to GPa. Figure 10 shows the time history of the Poisson s ratio at three chosen intervals in the fatigue test. The ab scissa shows the sample number of the data acquisition (proportional with time). Five full cycles correspond with 2.5 s (2 Hz). The behaviour is very similar with that in cyclic loadingunloading tests (see Fig. 6). The maximum value of the Poisson s ratio is clearly decreasing with increasing loading cycles, while the negative peaks are increasing as well. In Fig. 11, the evolution of the Poisson s ratio is again plotted against the longitudinal strain for the same sets of five cycles as shown in Fig. 10. The shape of the loadingunloading curves is very similar to the one showed in Fig. 7. It must be noticed as well that the Poisson s ratio shows a sharp decline during the first loading cycles. After only 600 cycles, the value has already decreased considerably. To be sure that the shape of the curves is not due to strain rate effects, the evolution of the Poisson s ratio is plotted against the longitudinal strain for the static tensile tests that were done before the fatigue testing and after 7500 cycles. Figure 12 shows that the initial Poisson s ratio is about 0.16 [ ], while after 7500 cycles, the shape of the curve appears again. It is important to stress the fact that the maximum applied strain during these static tensile tests was only (0.1%), in order to be sure that no damage was introduced into the specimen before fatigue testing. Indeed, this strain level is wel below the transverse failure strain of the 90 plies (0.0025, see Table 2). For the second fatigue test W 090 8, loading cycles were applied. The stress strain curve was measured before fatigue testing, but again only up till a very low axial strain of (0.1%). At two intermediate loading cycles, the fatigue test was stopped and the same static tensile test was repeated.
6 274 W. VAN PAEPEGEM et al. versus for [0 /90 ] 2s fatigue test W_090_7 versus time for [0 /90 ] 2s fatigue test W_090_8 [0 /90 ] 2s fatigue test W_090_8: cycle [0 /90 ] 2s fatigue test W_090_8: cycle [0 /90 ] 2s fatigue test W_090_8: cycle static [0 /90 ] 2s test W_090_7: cycle 0 intermediate static [0 /90 ] 2s test W_090_7: cycle Fig. 12 Evolution of the Poisson s ratio in function of the longitudinal strain for the initial and intermediate static tensile tests of the [0 /90 ] 2s fatigue test W Time Fig. 14 Time history of the Poisson s ratio for the [0 /90 ] 2s specimen W at three chosen intervals in the fatigue test. σ xx [MPa] Stressstrain curve for [0 /90 ] 2s fatigue test W_090_8 static [0 /90 ] 2s test W_090_8: cycle 0 intermediate static [0 /90 ] 2s test W_090_8: cycle 7500 intermediate static [0 /90 ] 2s test W_090_8: cycle = GPa = GPa = GPa Fig. 13 Stress strain curve for the initial and intermediate static tensile tests of the [0 /90 ] 2s fatigue test W versus for [0 /90 ] 2s fatigue test W_090_8 static [0 /90 ] 2s test IF4 static [0 /90 ] 2s test IF6 [0 /90 ] 2s fatigue test W_090_8: cycle [0 /90 ] 2s fatigue test W_090_8: cycle [0 /90 ] 2s fatigue test W_090_8: cycle Fig. 15 Evolution of the Poisson s ratio in function of the longitudinal strain for the 0 /90 ] 2s specimen W at three chosen intervals in the fatigue test. Figure 13 shows the stress strain curves before fatigue testing, and at cycle 7500 and cycle The initial stiffness of GPa decreases to GPa, and further to GPa. The comparison of the stiffness degradations in Fig. 13 and Fig. 9 is not straightforward due to the very different strain scale. In Fig. 13 a leastsquares linear fit to the full strain range [ ] has been done. If only the strain interval [ ] is used for determination of the Young s modulus, the values are and GPa, respectively. Figure 14 shows the time history of the Poisson s ratio for three chosen intervals in the fatigue test. The abscis shows again the sample number of the data acquisition, but the five plotted cycles correspond again with 2.5 s (2 Hz). The behaviour is very similar with that in cyclic loadingunloading tests (see Fig. 7). In Fig. 15, the evolution of the Poisson s ratio is again plotted against the longitudinal strain for the same sets of five cycles as shown in Fig. 14. The correspondence with Fig. 11 is again very good. It seems that both the maximum and minimum value of the Poisson s ratio are affected by the fatigue damage and could be a usable damage variable. Here again, the evolution of the Poisson s ratio versus longitudinal strain was measured under static loading conditions as well, to eliminate strain rate effects. However, the intermediate static tests were now performed up to a maximum strain of (0.6%), as opposed to Fig. 12. Figure 16 shows that the initial Poisson s ratio is now about [ ]. The scatter is quite large in the initial strain regime, due to the very low axial strains and even lower transverse strains ε yy. However, at an axial strain of
7 P O I S S O N S R AT I O A S A N I N D I C ATO R O F DA M AG E 0.001, the Poisson s ratio converges to a more or less constant value. In the intermediate static tests at cycles 7500 and , the same strain range [ ] as in the fatigue loading cycles has been applied. The same shape of the curve appears. More fatigue tests have been done that confirm the behaviour discussed above. Finally, some tests were taken up till final failure. The glass/epoxy composite is fully cracked then and turns white. After cycles failure occurs by fracture of the fibres. The typical damage patterns are shown in Fig. 17 for cycles (left) and at failure ( cycles). In this stage of severe damage, the evolution of the Poisson s ratio versus longitudinal strain still shows the same shape, but the amplitude is about 10 times smaller, as shown in Fig. 18. Some precaution is also necessary in this case. Due to the damaged surface, the bonding quality of the transverse strain gauge will have deteriorated, so that the strain transfer from the composite surface to the strain gauge is not reliable anymore. Perhaps a biaxial extensometer could be used to solve this problem. However, as the same shape still appears, it can be assumed that the measurements are still valid. CONCLUSIONS It has been demonstrated that both the amplitude and shape of the curve change when damage is present in a composite laminate. The static evolution of the Poisson s ratio is the envelope that encloses the cyclic curves. Also, the degradation of the Poisson s ratio is much larger than that of the stiffness. Further research is required to investigate the value of using the Poisson s ratio as a damage indicator for other material combinations than glass/epoxy. νxy versus εxx for [0 /90 ]2s fatigue test W_090_ εxx  intermediate static [0 /90 ]2s test W_090_4: cycle intermediate static [0 /90 ]2s test W_090_4: cycle νxy νxy νxy versus εxx for [0 /90 ]2s fatigue test W_0_90_ static [0 /90 ]2s test W_090_8: cycle 0 intermediate static [0 /90 ]2s test W_090_8: cycle 7500 intermediate static [0 /90 ]2s test W_090_8: cycle εxx Fig. 18 Evolution of the Poisson s ratio in function of the longitudinal strain εxx for the intermediate static tensile tests of the [0 /90 ]2s fatigue test W Fig. 17 Typical damage patterns in the [0 /90 ]2s specimens (a) close to failure, and (b) after failure. c 2007 Blackwell Publishing Ltd. Fatigue Fract Engng Mater Struct 30, Fig. 16 Evolution of the Poisson s ratio in function of the longitudinal strain for the initial and intermediate static tensile tests of the [0 /90 ]2s fatigue test W
8 276 W. VAN PAEPEGEM et al. Acknowledgements The author W. V. P. gratefully acknowledges his finance through a grant of the Fund for Scientific Research Flanders (F.W.O.) Procedings on CDROM. The authors also express their gratitude to Syncoglas for their support and technical collaboration. REFERENCES 1 Mallick, P. K. (1997) Composites Engineering Handbook. Marcel Dekker Inc., New York. 2 Herakovich, C. T. (1998) Mechanics of Fibrous Composites. John Wiley & Sons, Inc., New York. 3 Schulte, K., Baron, Ch., Neubert, H., et al (1985) Damage development in carbon fibre epoxy laminates : Cyclic loading. In : Proceedings of the MRSsymposium Advanced Materials for Transport, November 1985, Strassbourg, pp Schulte, K., Reese, E. and Chou, T.W. (1987) Fatigue behaviour and damage development in woven fabric and hybrid fabric composites. In : Sixth International Conference on Composite Materials (ICCMVI) & Second European Conference on Composite Materials (ECCMII) (Edited by F. L. Matthews, N. C. R. Buskell, J. M. Hodgkinson, and J. Morton) Vol. 4. Proceedings, July 1987, Elsevier, London, UK, pp Schulte, K. (1984) Stiffness reduction and development of longitudinal cracks during fatigue loading of composite laminates. In : Mechanical characterisation of load bearing fibre composite laminates. Proceedings of the European Mechanics Colloquium 182, August 1984, Brussels, (Edited by A. H. Cardon and G. Verchery) Elsevier, Belgium, pp Fujii, T., Amijima, S. and Okubo, K. (1993) Microscopic fatigue processes in a plainweave glassfibre composite. Comp. Sci. Technol. 49, Pandita, S. D., Huysmans, G., Wevers, M. and Verpoest, I. (2000) Tensile fatigue behaviour of glassplain weave fabric composites in the on and offaxis directions. Proceedings of the Fifth International Conference on Textile Composites, Leuven, Belgium, September Sidoroff, F. and Subagio, B. (1987) Fatigue damage modelling of composite materials from bending tests. In : Sixth International Conference on Composite Materials (ICCMVI) & Second European Conference on Composite Materials (ECCMII) (Edited by F. L. Matthews, N. C. R. Buskell, J. M. Hodgkinson, and J. Morton) Vol. 4. Proceedings, July 1987, Elsevier, London, UK, pp Vieillevigne, S., Jeulin, D., Renard, J. and Sicot, N. (1997) Modelling of the fatigue behaviour of a unidirectional glass epoxy composite submitted to fatigue loadings. In: International Conference on fatigue of composites (Edited by S. Degallaix, C. Bathias and R. Fougères). Proceedings, 35 June 1997, La Société Française de Métallurgie et de Matériaux, Paris, France, pp Kawai, M. (1999) Damage mechanics model for offaxis fatigue behavior of unidirectional carbon fiberreinforced composites at room and high temperatures. In: Proceedings of the Twelfth International Conference on Composite Materials (ICCM12) (Edited by T. Massard and A. Vautrin). Paris, France, 5 9 July 1999, pp Hwang, W. and Han, K. S. (1986) Fatigue of composites  Fatigue modulus concept and life prediction. J. Comp. Mater. 20, Hwang, W. and Han, K. S. (1986) Cumulative damage models and multistress fatigue life prediction. J. Comp. Mater. 20, Whitworth, H. A. (1987) Modelling stiffness reduction of graphite epoxy composite laminates. J. Comp. Mater. 21, Yang, J. N., Jones, D. L., Yang, S. H. and Meskini, A. (1990) A stiffness degradation model for graphite/epoxy laminates. J. Comp. Mater. 24, Brøndsted, P., Andersen, S. I. and Lilholt, H. (1997) Fatigue damage accumulation and lifetime prediction of GFRP materials under block loading and stochastic loading. In : Polymeric Composites  Expanding the Limits. Proceedings of the 18th Risø International Symposium on Materials Science, 15 September 1997 (Edited by S. I. Andersen, P. Brøndsted, H. Lilholt, Aa. Lystrup, J. T. Rheinländer, B. F. Sørensen and H. Toftegaard). Risø International Laboratory, Roskilde, Denmark, pp Brondsted, P., Lilholt, H. and Andersen, S. I. (1997) Fatigue damage prediction by measurements of the stiffness degradation in polymer matrix composites. In : International Conference on fatigue of composites (Edited by S. Degallaix, C. Bathias and R. Fougères) Proceedings, 3 5 June 1997, La Société Française de Métallurgie et de Matériaux, Paris, France, pp Bandoh, S., Matsumura, K., Zako, M., Shiino, T. and Kurashiki, T. (2001) On the detection of fatigue damage in CFRP by measuring Poisson s ratio. In: Eighth International Conference on Composites Engineering (ICCE/8) (Edited by D. Hui) Proceedings. Tenerife, Spain, 5 11 August 2001, pp Pidaparti, R. M. and Vogt, A. (2002) Experimental investigation of Poisson s ratio as a damage parameter for bone fatigue. J. Biomed. Mater. Res. Part A 59, Sol, H. and de Wilde, W. P. (1988) Identification of elastic properties of composite materials using resonant frequencies. In : Proceedings of the International Conference Computer Aided Design in Composite Material Technology (Edited by C.A. Brebbia, W. P. de Wilde and W. R. Blain) 1988, SpringerVerlag, Southampton, pp Sol, H. (1990) Identification of the complex moduli of composite materials by a mixed numerical/experimental method. In : Proceedings of the second International Conference on Computer Aided Design in Composite Material Technology (Edited by W. P. de Wilde and W. R. Blain) April 1990, SpringerVerlag, Brussels, pp Van Paepegem, W., De Baere, I. and Degrieck, J. (2005) Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part I: Experimental results. Comp. Sci. Technol. 66, Van Paepegem, W., De Baere, I. and Degrieck, J. (2005) Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations. Comp. Sci. Technol. 66,
International Journal of Fatigue
International Journal of Fatigue 32 (2010) 184 196 Contents lists available at ScienceDirect International Journal of Fatigue journal homepage: www.elsevier.com/locate/ijfatigue Monitoring quasistatic
More informationExperimental setup for and numerical modelling of bending fatigue experiments on plain woven glass/epoxy composites
Experimental setup for and numerical modelling of bending fatigue experiments on plain woven glass/epoxy composites W. Van Paepegem a* and J. Degrieck b a Research Assistant of the Fund for Scientific
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationNonlinear correction to the bending stiffness of a damaged composite beam
Van Paepegem, W., Decaene, R. and Degrieck, J. (5). Nonlinear correction to te bending stiffness of a damaged composite beam. Nonlinear correction to te bending stiffness of a damaged composite beam W.
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationMESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE
MESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE S. Daggumati a*,i. De Baere a, W. Van Paepegem a, J. Degrieck a, J. Xu b, S.V. Lomov b, I. Verpoest b a Ghent University, Dept. of
More informationProbabilistic fatigue life prediction of multidirectional composite laminates
Composite Structures 69 () 9 www.elsevier.com/locate/compstruct Probabilistic fatigue life prediction of multidirectional composite laminates Yongming Liu, Sankaran Mahadevan * Department of Civil and
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationScienceDirect. Fatigue behaviour of a thermoplastic composite reinforced with woven glass fibres for automotive application
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 133 (215 ) 136 147 6th Fatigue Design conference, Fatigue Design 215 Fatigue behaviour of a thermoplastic composite reinforced
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationEXPERIMENTAL AND THEORETICAL STUDY OF THE DAMAGE ONSET IN BIAXIAL CRUCIFORM SPECIMENS UNDER STATIC AND HYSTERESIS LOADING
EXPERIMENTAL AND THEORETICAL STUDY OF THE DAMAGE ONSET IN BIAXIAL CRUCIFORM SPECIMENS UNDER STATIC AND HYSTERESIS LOADING E. Lamkanfi a,1, C. Ramault 2, A. Makris 2, W. Van Paepegem 1, J. Degrieck 1, D.
More informationImplementation of fatigue model for unidirectional laminate based on finite element analysis: theory and practice
Focussed on Multiaxial Fatigue and Fracture Implementation of fatigue model for unidirectional laminate based on finite element analysis: theory and practice D. CarrellaPayan, B. Magneville, M. Hack,
More informationMATERIALS AND METHODS
Modelling the Nonlinear Shear Stress Strain Behavior of a Carbon Fabric Reinforced Polyphenylene Sulphide From Rail Shear and [(458,2458)] 4s Tensile Test Ives De Baere, Wim Van Paepegem, Joris Degrieck
More informationPrediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach
Prediction of the Ultimate Strength of Composite Laminates Under InPlane Loading Prediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach Tae Jin
More informationEFFECT OF THERMAL FATIGUE ON INTRALAMINAR CRACKING IN LAMINATES LOADED IN TENSION
EFFECT OF THERMAL FATIGUE ON INTRALAMINAR CRACKING IN LAMINATES LOADED IN TENSION J.Varna and R.Joffe Dept of Applied Physics and Mechanical Engineering Lulea University of Technology, SE 97187, Lulea,
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationTENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES
TENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES C. Qian 1 *, R. P. L. Nijssen 1, D. D. Samborsky 2, C.Kassapoglou 3, Z. Gürdal 3, G. Q. Zhang 4 1 Knowledge Centre Wind turbine Materials and
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationComparison of different identification techniques for measurement of quasizero Poisson s ratio of fabricreinforced laminates
Composites: Part A 38 (2007) 2047 2054 www.elsevier.com/locate/compositesa Comparison of different identification techniques for measurement of quasizero Poisson s ratio of fabricreinforced laminates
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationApplication of Biaxial FBG Sensors to Monitor Poisson s Ratio of Composites as Damage Index
8th European Workshop On Structural Health Monitoring (EWSHM 216, 58 July 216, Spain, Bilbao www.ndt.net/app.ewshm216 Application of Biaxial FBG Sensors to Monitor Poisson s Ratio of Composites as Damage
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationIn Situ Ultrasonic NDT of Fracture and Fatigue in Composites
ECNDT 26  Mo.2.6.5 In Situ Ultrasonic NDT of Fracture and Fatigue in Composites I. SOLODOV, K. PFLEIDERER, and G. BUSSE Institute for Polymer Testing and Polymer Science (IKP), Nondestructive Testing
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationFatigue Damage Modelling of Fibrereinforced Composite Materials: Review
Degrieck, J. and Van Paepegem, W. (1). Fatigue Damage Modelling of FibreReinforced Composite Materials: Review. Applied Mechanics Reviews, 54(4), 793. Fatigue Damage Modelling of Fibrereinforced Composite
More informationDEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL
DEVELOPMENT OF THERMOELASTIC STRESS ANALYSIS AS A NONDESTRUCTIVE EVALUATION TOOL S. Quinn*, R.K. Fruehmann and J.M. DulieuBarton School of Engineering Sciences University of Southampton Southampton SO17
More informationKeywords: Adhesively bonded joint, laminates, CFRP, stacking sequence
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS GLOBAL AND LOCAL INFLUENCE OF STACKING SEQUENCE ON THE STRENGTH OF ADHESIVELY BONDED JOINTS OF CFRP LAMINATES J. Rousseau*, P. Satthamnuwong DRIVE,
More informationIDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE
IDENTIFICATION OF THE ELASTIC PROPERTIES ON COMPOSITE MATERIALS AS A FUNCTION OF TEMPERATURE Hugo Sol, hugos@vub.ac.be Massimo Bottiglieri, Massimo.Bottiglieri@vub.ac.be Department Mechanics of Materials
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationEvaluation of inplane orthotropic elastic constants of paper and paperboard
Evaluation of inplane orthotropic elastic constants of paper and paperboard T. Yokoyama and K. Nakai Department of Mechanical Engineering, Okayama University of Science  Ridaicho, Okayama 75, Japan
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationProject MMS13 Task 5 Report No 3 (M6/D3)
Project MMS13 Task 5 Report No 3 (M6/D3) Material Data Requirements and Recommended Test Methods for the Predictive Modelling of Defect Criticality in Composite Material Systems M R L Gower and G D Sims
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationA fatigue design methodology for GRP composites in offshore underwater applications
A fatigue design methodology for GRP composites in offshore underwater applications Dr P. A. FRIEZE P A F A Consulting Engineers Limited, Hampton, Middx, UK INTRODUCTION Norsk Hydro Troll C field  floating
More informationSCALING EFFECTS IN THE LOW VELOCITY IMPACT RESPONSE OF FIBRE METAL
SCALING EFFECTS IN THE LOW VELOCITY IMPACT RESPONSE OF FIBRE METAL LAMINATES J. G. Carrillo 1, S. McKown 1, M. Mujib 1 and W. J. Cantwell 1. R. Day 2 1 Department of Engineering, University of Liverpool,
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationAnalysis of nonlinear shear deformations in CFRP and GFRP textile laminates
Loughborough University Institutional Repository Analysis of nonlinear shear deformations in CFRP and GFRP textile laminates This item was submitted to Loughborough University's Institutional Repository
More informationSTRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES
ECCM1616 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 214 STRUCTURAL EFFICIENCY VIA MINIMISATION OF ELASTIC ENERGY IN DAMAGE TOLERANT LAMINATES M. Nielsen a, A. T. Rhead a,
More informationINVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT
INVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT Andreas Endruweit, Dhiren K. Modi and Andrew C. Long School of Mechanical, Materials and Manufacturing Engineering, University of
More information1. Introduction. 2. Testing strategy. Daniel HUELSBUSCH 1, Frank WALTHER 1
6th International Symposium on NDT in Aerospace, 1214th November 2014, Madrid, Spain  www.ndt.net/app.aerondt2014 More Info at Open Access Database www.ndt.net/?id=16947 Damage detection and fatigue
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationMesoscale Modeling of Static and Fatigue Damage in Woven Composite Materials with Finite Element Method
Mesoscale Modeling of Static and Fatigue Damage in Woven Composite Materials with Finite Element Method J. Xu a*, SV. Lomov a, I. Verpoest a, S. Daggumati b, W. Van Paepegem b, J. Degrieck b a Katholieke
More informationNonlinearities in mechanical behavior of textile composites
Composite Structures 71 (25) 61 67 www.elsevier.com/locate/compstruct Nonlinearities in mechanical behavior of textile composites Enrico DÕAmato Energetics Departement, L Aquila University, 674 Monteluco
More informationSPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION
AIAA225 SPECTRUM FATIGUE LIFETIME AND RESIDUAL STRENGTH FOR FIBERGLASS LAMINATES IN TENSION Neil Wahl Montana Tech of The University of Montana Butte, Montana 597 Daniel Samborsky John Mandell Douglas
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More informationA Constitutive Model for DYNEEMA UD composites
A Constitutive Model for DYNEEMA UD composites L Iannucci 1, D J Pope 2, M Dalzell 2 1 Imperial College, Department of Aeronautics London, SW7 2AZ l.iannucci@imperial.ac.uk 2 Dstl, Porton Down, Salisbury,
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationFOLDING OF WOVEN COMPOSITE STRUCTURES
FOLDING OF WOVEN COMPOSITE STRUCTURES J.C.H. Yee and S. Pellegrino 1 Department of Engineering, University of Cambridge Trumpington Street, Cambridge CB2 1PZ, UK ABSTRACT This paper investigates oneply
More informationAccelerated Testing Methodology for Long Term Durability of CFRP
IFREMERONR Workshop on Durability of Composites in a Marine Environment August 23 24, 22 IFREMER Centre, Nantes, France Accelerated esting Methodology for Long erm Durability of CFRP Masayuki Nakada*,
More informationA Fracture Mechanics Approach to the Water Jet Drilling of Composite Materials. Y. AH Mashal* and M. W. Algrafi
A Fracture Mechanics Approach to the Water Jet Drilling of Composite Materials Y. AH Mashal* and M. W. Algrafi Department of Mechanical Engineering, College of Engineering, Taibah University, KSA prof.yosry@gmail.com
More informationComposites Science and Technology
Composites Science and Technology 7 (1) 194 1941 Contents lists available at ScienceDirect Composites Science and Technology journal homepage: www.elsevier.com/locate/compscitech Local damage in a 5harness
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationModelling of multiaxial ultimate elastic wall stress (UEWS) test for glass fibre reinforced epoxy (GRE) composite pipes
pplied Mechanics and Materials Vol. 367 (013) pp 113117 Online available since 013/ug/16 at www.scientific.net (013) Trans Tech Publications, Switzerland doi:10.408/www.scientific.net/mm.367.113 Modelling
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationAssessment Methods of Mechanical Properties of Composite Materials
Mechanics and Mechanical Engineering Vol. 21, No. 4 (2017) 1005 1018 c Lodz University of Technology Assessment Methods of Mechanical Properties of Composite Materials Monika Kamocka Radoslaw J. Mania
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationNumerical Evaluation of Fracture in Woven Composites by Using Properties of Unidirectional Type for modelling
J. Basic. Appl. Sci. Res., 2(12)1320213209, 2012 2012, TextRoad Publication ISSN 20904304 Journal of Basic and Applied Scientific Research www.textroad.com Numerical Evaluation of Fracture in Woven Composites
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More information2 Experiment of GFRP bolt
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FATIGUE LIFE EVALUATION OF BOLT MADE OF WOVEN FABRIC FRP Takeshi INOUE*, Hiroaki NAKAI**, Tetsusei KURASHIKI**, Masaru ZAKO**, Yuji KOMETANI*** *Graduate
More informationA STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS
Xi an, 225 th August 217 A STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS LI Zhongyang 1, LI Dong 2 Mailbox7235, Yanliang District, Xian, China, Email: zhongyangli@live.com Keywords:
More informationAgnieszka Bondyra, Pawe Gotowicki
Journal of KONES Powertrain and Transport, Vol. 17, No. 1 21 INFLUENCE OF A CROSSHEAD RATE AND A NUMBER OF STRESS CYCLES ON MEASUREMENT RESULTS IN THE INPLANE SHEAR TEST FOR A CROSSPLY VINYLESTERCARBON
More informationEffects with a matrix crack on monitoring by electrical resistance method
Adv. Composite Mater., Vol. 13, No. 2, pp. 107 120 (2004) VSP 2004. Also available online  www.vsppub.com Effects with a matrix crack on monitoring by electrical resistance method AKIRA TODOROKI, MIHO
More informationThe science of elasticity
The science of elasticity In 1676 Hooke realized that 1.Every kind of solid changes shape when a mechanical force acts on it. 2.It is this change of shape which enables the solid to supply the reaction
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationProgressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study
Progressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study Progressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study Md
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationThermomechanical Studies in Glass/Epoxy Composite Specimen during Tensile Loading
Thermomechanical Studies in Glass/Epoxy Composite Specimen during Tensile Loading K. M. Mohamed Muneer, Raghu V. Prakash, and Krishnan Balasubramaniam Abstract This paper presents the results of thermomechanical
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationCalibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques
9 th International LSDYNA Users Conference Optimization Calibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques Stefano Magistrali*, Marco
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationRELIABILITY OF COMPOSITE STRUCTURES  IMPACT LOADING 
RELIABILITY OF COMPOSITE STRUCTURES  IMPACT LOADING  L.Guillaumat 1 1 LA.M.E.F.E.N.S.A.M. Esplanade des Arts et Métiers 33405 Talence Cedex  FRANCE SUMMARY: This paper deals with a method to study
More informationSTRESS ANALYSIS OF BONDED JOINTS IN PULTRUDED GRP COMPONENTS
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF BONDED JOINTS IN PULTRUDED GRP COMPONENTS S.W. Boyd*, J. M. DulieuBarton*, O. T. Thomsen**, A.Gherardi* [J.M. DulieuBarton]: janice@soton.ac.uk
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationEFFECTS OF MODELING ASSUMPTIONS ON THE ACCURACY OF SPECTRUM FATIGUE LIFETIME PREDICTIONS FOR A FIBERGLASS LAMINATE
EFFECTS OF MODELING ASSUMPTIONS ON THE ACCURACY OF SPECTRUM FATIGUE LIFETIME PREDICTIONS FOR A FIBERGLASS LAMINATE Neil Wahl Montana Tech of The University of Montana Butte, Montana 5970 Daniel Samborsky
More information